HAL Id: hal-01171774
Submitted on 6 Jul 2015
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Pseudocapacitive oxide materials for high-rate
electrochemical energy storage
Veronica Augustyn, Patrice Simon, Bruce Dunn
To cite this version:
Veronica Augustyn, Patrice Simon, Bruce Dunn. Pseudocapacitive oxide materials for high-rate
elec-trochemical energy storage. Energy & Environmental Science, Royal Society of Chemistry, 2014, vol.
7 (n° 5), pp. 1597-1614. �10.1039/c3ee44164d�. �hal-01171774�
To link to this article : DOI:10.1039/c3ee44164d
This is an author-deposited version published in:
Eprints ID: 13900
To cite this version:
Augustyn, Veronica and Simon, Patrice and Dunn, Bruce Pseudocapacitive
oxide materials for high-rate electrochemical energy storage. (2014) Energy &
Environmental Science, vol. 7 (n° 5). pp. 1597-1614. ISSN 1754-5692
OATAO is an open access repository that collects the work of Toulouse researchers
and makes it freely available over the web where possible.
Any correspondence concerning this service should be sent to the repository
Pseudocapacitive oxide materials for high-rate
electrochemical energy storage
Veronica Augustyn,†aPatrice Simonbcand Bruce Dunn*a
Electrochemical energy storage technology is based on devices capable of exhibiting high energy density (batteries) or high power density (electrochemical capacitors). There is a growing need, for current and near-future applications, where both high energy and high power densities are required in the same material. Pseudocapacitance, a faradaic process involving surface or near surface redox reactions, oﬀers a means of achieving high energy density at high charge–discharge rates. Here, we focus on the pseudocapacitive properties of transition metal oxides. First, we introduce pseudocapacitance and describe its electrochemical features. Then, we review the most relevant pseudocapacitive materials in aqueous and non-aqueous electrolytes. The major challenges for pseudocapacitive materials along with a future outlook are detailed at the end.
The importance of electrical energy storage will continue to grow as markets for consumer electronics and electrication of transportation expand and energy storage systems for renewable energy sources begin to emerge. There is a need, particularly with transportation and grid storage applications, where large amounts of energy need to be delivered or accepted quickly, within seconds or minutes. Although carbon based electrochemical capacitors possess the required power density, their relatively low energy density limits their usefulness for these applications. Instead, transition metal oxides that exhibit pseudocapacitance are very attractive. Pseudocapacitance occurs when reversible redox reactions occur at or near the surface of an electrode material and are fast enough so that the device's electrochemical features are those of a carbon-based capacitor, but with signicantly higher capacitances. It is important to recognize that pseudo-capacitance in materials is a relatively new property, with the rst materials identied in the 1970's. Thus, both materials systems and electrochemical char-acteristics which lead to high energy density at high charge–discharge rates are still being identied. To date, transition metal oxides exhibit the widest range of materials with pseudocapacitive behavior. By selecting the proper transition metal oxide, utilizing the most eﬀective electrode architecture, and analyzing the electrochemical behavior for pseudocapacitive behavior, such materials are expected to become the basis for electrochemical energy storage devices which oﬀer high energy density at high rates.
Electrochemical energy storage (EES) in the form of batteries and electrochemical capacitors is widely used for powering the now-ubiquitous portable electronics in our society and for the electrication of the transportation sector. The emerging need to overhaul the power grid in many developed countries combined with the expected rise in global energy needs (arising at least partly from the need to electrify developing countries) over the coming decades have brought another application for EES, the coupling of these technologies with renewable energy sources like solar and wind for powering the electrical grid. While opportunities for EES abound, there are several
challenges for these devices that are rooted primarily in nding materials that are better at both storing and delivering large amounts of energy. These functions would ideally be performed by abundant, non-toxic materials in order to also lower the cost and increase the safety of EES devices in consumer products as well as in stationary power.
The current success of EES is in large part due to the use of transition metal oxides in one or both electrodes. This review is concerned with transition metal oxide materials that exhibit pseudocapacitance, which arises when reversible redox reac-tions occur at or near the surface of a material in contact with an electrolyte, or when these reactions are not limited by solid-state ion diﬀusion. The behavior can exist in both aqueous and non-aqueous electrolytes and can be intrinsic to the material, or extrinsic. The signicant diﬀerence between battery and pseudocapacitive materials is that the charging and discharging behavior of pseudocapacitive materials occurs on the order of seconds and minutes. Thus a strong motiva-tion for studying and developing pseudocapacitance is that it leads to both high energy and high power densities in the same material.
aDepartment of Materials Science and Engineering, University of California Los
Angeles, Los Angeles, CA 90095-1595, USA. E-mail: email@example.com
bDepartment of Materials Science, Universit´e Paul Sabatier, CIRIMAT UMR CNRS
5085, Toulouse, France
cR´eseau sur le Stockage Electrochimique de l'Energie (RS2E), FR CNRS 3459, France
†Present address: Texas Materials Institute, The University of Texas at Austin, Austin, TX 78712-1591, USA.
Fig. 1 shows the specic energy vs. charging time plot for an electric double layer capacitor (EDLC) and a high-rate lithium-ion battery.1This plot clearly demonstrates that a lithium-ion
battery optimized for high-power exhibits constant energy density for discharge times >10 minutes. At shorter timescales, this energy decreases due to the various resistive losses within a battery cell, mainly stemming from sluggish electron and ion transport. These resistive losses, particularly at high rates, give rise to heat generation which can lead to serious safety prob-lems such as thermal runaway.2On the other hand,
commer-cially-available EDLCs exhibit constant energy densities for all timescales but their total stored energy is low. In between the regimes where EDLCs and lithium-ion batteries exhibit their best performance is a time domain (!10 s to 10 minutes) that appears well-suited for the pseudocapacitive materials described in this review.
Such high-rate EES is desirable for numerous applications where a large amount of energy needs to be either stored or delivered quickly. These include kinetic energy harvesting in seaports3or with regenerative braking;4pulse power in
commu-nication devices;5and power quality applications in the power
grid.6In addition, shorter charging times would be very
conve-nient for portable devices and especially for electric vehicles. This review is organized into three sections: (a) the back-ground, which details the historical development of pseudoca-pacitance, the mechanisms that give rise to pseudocapseudoca-pacitance, and the electrochemical features of this behavior; (b) materials that exhibit pseudocapacitance in aqueous electrolytes; and (c) materials that exhibit pseudocapacitance in non-aqueous elec-trolytes. In order to aid in the comparison of the diﬀerent materials, capacity and capacitance values as well as the time of Fig. 1 Energy vs. charging time for an EDLC and a lithium-ion battery.1
The region between!10 s and 10 minutes represents the time domain where high-rate pseudocapacitive materials could oﬀer higher energy and power densities than lithium-ion batteries and EDLCs. Repro-duced by permission of The Electrochemical Society.
Patrice Simon is Professor of Materials Science at the Uni-versit´e Paul Sabatier in Tou-louse, France. His research interests are in the synthesis and electrochemical characterization of materials for supercapacitors and batteries. An important part of his work focuses on the development of porous carbon structures and the study of ion connement and dynamics in carbon micropores. Professor Simon has received several awards for his work including an Advanced Grant from the European Research Council (ERC) in 2011 and the Tajima Prize of the International Electrochemical Society (2009). Together with Prof. Jean-Marie Tarascon, he leads the French network on Electrochemical Energy Storage (RS2E).
Bruce Dunn is the Nippon Sheet Glass Professor of Materials Science and Engineering at UCLA. Prior to joining UCLA in 1981, he was a staﬀ scientist at the General Electric Research Laboratory. His research inter-ests are in the synthesis of inor-ganic and organic/inorganic materials, and the design of their electrochemical, optical and biochemical properties. His current programs in electro-chemistry include creating pseudocapacitive materials and the fabrication of three-dimensional batteries. Professor Dunn has received a number of honors including a Fulbright research fellowship, invited professorships at the University of Paris, the University of Bordeaux and two awards from the Department of Energy for Outstanding Research in Materials Science. He is a Fellow of the American Ceramic Society and the Materials Research Society.
Veronica Augustyn received her Ph.D. degree in Materials Science and Engineering under the supervision of Prof. Bruce Dunn from the University of California, Los Angeles, in 2013. She is currently a Postdoctoral Fellow at the University of Texas at Austin, working in the laboratory of Prof. Arumugam Manthiram. Her current research interests include the design, synthesis, and characterization of novel transi-tion-metal based materials for electrochemical energy storage and electrocatalysis.
the experiment are reported as oen as possible. The incorpo-ration of pseudocapacitive materials in electrode structures can result in dramatic diﬀerences for certain materials, and this is highlighted when appropriate. While it has been known for some time what electrochemical features are indicative of pseudoca-pacitance, a clear understanding of the mechanisms and the manner in which these depend upon the redox chemistry and structure of the material is an area of active investigation.
While the idea that charges could accumulate on solids was known since ancient times, (dating back to the Greek word for amber – electron)7
the rst patent for an electrochemical capacitor was not led until 1957 by General Electric.8This was a
relatively late entry into the energy storage eld because, with the exception of the lithium-ion battery, most energy storage devices were invented by the end of the 19th
–early 20thcentury. The patent contains an interesting statement: “it is not positively known exactly what takes place when the devices [.] are used as energy storing devices”. It should be noted that the need for a high surface area electrode was identied. Today it is known that such devices store charge through the adsorption of electrolyte ions onto the surfaces of electried materials, and that carbons are ideal materials due to the combination of high conductivity, large surface areas, and low density. This type of charge storage is electrostatic and no redox reactions are involved. Such devices are called electric double-layer capacitors (EDLCs) and commercial devices can store between 3 and 6 W h kg"1.9
The eld of EDLCs has been the subject of numerous reviews over the past few years.10–12A major research objective in the eld
of EDLCs is to understand the dependence of electrode area, including pore structure, on the capacitance.13Currently, the best
carbon materials achieve double-layer capacitances of approxi-mately 150 F g"1for optimum carbon pore sizes in ionic liquid electrolytes.14 Strategies for improving the energy densities of
EDLCs include functionalizing the surface with nitrogen and oxygen groups,15utilizing pore sizes that match the electrolyte
ion size,16 using redox-active species in the electrolyte,17 or
designing ionic liquid mixtures for improving the cell voltage and temperature range.18The prospect of using graphene for EDLCs
has generated considerable interest in the community. The high surface area of graphene has led to specic capacitances in the range of 100–250 F g"1.19,20However, because of the nanoscale
sheet-like morphology of these materials, there is a concern that the gravimetric-normalized capacitance may not be a useful metric.21
Nonetheless, graphene has been particularly eﬀective in the development of exible device architectures for EDLCs. 2.1. Development of pseudocapacitance in RuO2
In 1971, a new type of electrochemical capacitance was discov-ered in RuO2, termed pseudocapacitance because it involved
faradaic charge-transfer reactions.22The storage of protons from
the electrolyte resulted in a faradaic charge-transfer reaction on the RuO2thin lm electrode. Despite the faradaic nature of the
charge storage process, the cyclic voltammogram (CV) was that of
a capacitor – i.e. rectangular in shape (Fig. 2). While this rst report resulted in low gravimetric capacitance values (only 4–7% of the Ru4+atoms participated in the redox reaction), it demon-strated the unique electrochemical features of pseudocapacitive processes. This study also demonstrated the need for a porous and hydrous oxide as the bulk, single-crystal material did not exhibit a rectangular CV. Subsequent studies improved the capacitance to over 700 F g"1(700 C g"1, !8.3 min) by identifying
the importance of structural water (specically, RuO2$nH2O
where x ¼ 0.5)23 and a porous, nanoscale architecture.24The
storage of protons by hydrated RuO2can be expressed as:25
RuOx(OH)y+ dH++ de"4 RuOx"d(OH)y+d (1)
and when d ¼ 2 this results in a maximum theoretical capaci-tance of 1450 F g"1of RuO2(1360 F g"1of RuO2$0.5H2O) over a
1 V window.
RuO2$0.5H2O exhibits four unique features that enable rapid
faradaic reactions with high capacitance: (1) the redox behavior of the Ru4+cation that allows for faradaic energy storage; (2) the metallic conductivity of RuO2 that allows for rapid electron
transport; (3) the presence of structural water that enables rapid proton transport within the so-called “inner surface”; and (4) a large “outer” surface area that decreases diﬀusion distances. Unfortunately, the high cost of ruthenium (currently at !2000 USD per kg) makes devices based on RuO2 impractical for
widespread application, except in small-size devices such as Fig. 2 Cyclic voltammetry at 40 mV s"1of a RuO2thin ﬁlm (top) and
single crystal (bottom) in 1 M HClO4. This ﬁrst investigation of the
unique behavior of RuO2ﬁlms demonstrated how redox reactions at
the surface can give rise to electrochemical features of capacitors. Reprinted from ref. 22, with permission from Elsevier.
microsupercapacitors. Nevertheless, the behavior of hydrous RuO2 rst demonstrated that in certain systems, reversible
faradaic reactions can result in similar electrochemical features as those of a capacitor. The study of RuO2 also led to the
understanding of what constitutes an ideal pseudocapacitive material in aqueous electrolytes.
2.2. Types of pseudocapacitive mechanisms
Conway identied several faradaic mechanisms that can result in capacitive electrochemical features:7 (1) underpotential
deposition, (2) redox pseudocapacitance (as in RuO2$nH2O),
and (3) intercalation pseudocapacitance. These processes are illustrated in Fig. 3. Underpotential deposition occurs when metal ions form an adsorbed monolayer at a diﬀerent metal's surface well above their redox potential. One classic example of underpotential deposition is that of lead on the surface of a gold electrode.26 Redox pseudocapacitance occurs when ions are
electrochemically adsorbed onto the surface or near surface of a material with a concomitant faradaic charge-transfer. Interca-lation pseudocapacitance occurs when ions intercalate into the tunnels or layers of a redox-active material accompanied by a faradaic charge-transfer with no crystallographic phase change. These three mechanisms occur due to diﬀerent physical processes and with diﬀerent types of materials; the similarity in the electrochemical signatures occurs due to the relationship between potential and the extent of charge that develops as a result of adsorption/desorption processes at the electrode/ electrolyte interface or within the inner surface of a material:27
E! E0"RT nF ln ! X 1" X " (2) here, E is the potential (V), R is the ideal gas constant (8.314 J
mol"1K"1), T is the temperature (K), n is the number of
elec-trons, F is the Faraday constant (96 485 C mol"1), and X is the extent of fractional coverage of the surface or inner structure. In eqn (2), a capacitance (C; F g"1) may be dened in regions where
the plot of E vs. X is linear: C¼!nF
m " X
where m is the molecular weight of the active material. Since the plot of E vs. X is not entirely linear as in a capacitor,
the capacitance is not always constant and so it is termed pseudocapacitance.
While the above relationship describes the thermodynamic basis for pseudocapacitance, the utility of such materials for energy storage is in their kinetic behavior. This stems from the fact that reactions that occur at the surface, or are limited by the surface, are not limited by solid-state diﬀusion and therefore exhibit high rate capability. This is an important diﬀerence between transition metal oxides that exhibit pseudocapacitive behavior and those that do not. The latter are materials that are utilized in rechargeable batteries, where the use of the bulk solid state to store charge results in high energy densities. However, in these devices the power capability is limited by the solid-state diﬀusion within the cathode and anode active materials.2
2.3. Electrochemical features of pseudocapacitance
Pseudocapacitance can result from various processes as mentioned previously. Electrochemically, pseudocapacitance gives rise to specic features as presented in this section. We describe pseudocapacitive energy storage on the basis of its response to (a) a voltage sweep, as in cyclic voltammetry; (b) constant current, as in galvanostatic cycling, and (c) alternating current, as in impedance spectroscopy.
In a cyclic voltammetry experiment, the timescale of the experiment is controlled by the sweep rate (v, mV s"1). The
current response to an applied sweep rate will vary depending on whether the redox reaction is diﬀusion-controlled or surface-controlled (capacitive). For a redox reaction limited by semi-innite linear diﬀusion, the current response varies with v1/2; for a capacitive process, the current varies directly with v. Therefore, for any material the following general relationship may be written for the current at a particular potential:28
i(V)¼ k1v 1/2
+ k2v (4)
Solving for the values of k1and k2at each potential allows for
the separation of the diﬀusion and capacitive currents. Care should be taken in utilizing this mathematical treatment as the current relationships do not establish the mechanism: this should be corroborated with other characterization techniques. The technique has been utilized to evaluate the performance of novel nanostructured materials,29–32as shown in the example in Fig. 4.
A related analysis rst suggested by Trasatti, et al.34describes
the relationship between the capacity and the sweep rate. Capacity that is occurring due to surface processes will be constant with the sweep rate and thus will always be present, even at high sweep rates. Capacity that occurs due to processes limited by semi-innite linear diﬀusion will vary with v"1/2. In the following equation, the capacitive contribution is represented by Qv¼N, which is the innite-sweep rate capacity; the diﬀusion-controlled capacity is the remaining contribution, and is limited by v"1/2:
Q¼ Qv¼N+ constant (v"1/2) (5)
An example of this analysis applied to a coating of NiCo2O4is
shown in Fig. 5. In this plot of capacity vs. v"1/2, the extrapola-tion of the linear t to the data to the y-intercept (v"1/2¼ 0) gives Fig. 3 Diﬀerent types of reversible redox mechanisms that give rise to
pseudocapacitance: (a) underpotential deposition, (b) redox pseudo-capacitance, and (c) intercalation pseudocapacitance.
Qv¼N. Here, Qv¼N is !10.5 mC cm"2 which represents the contribution of the so-called outer surface of NiCo2O4to the
charge storage. At 5 mV s"1, the outer surface of NiCo2O4
contributes !62% of the total capacity.
Another feature of rapid energy storage is the relationship between peak potential and sweep rate.36In a capacitive system,
there is very little potential hysteresis between the charging and discharging steps particularly for slow charge–discharge times. In a cyclic voltammetry experiment, this translates into a small or no potential diﬀerence between the anodic and cathodic peak currents at slow sweep rates, as shown in Fig. 6 for a lm of 30 nm Nb2O5nanocrystals. A small potential diﬀerence in a Nernstian
process also indicates that the reaction is reversible and in such a reaction, the peak voltage diﬀerence is 59 mV n"1, where n is the
number of electrons involved.37This behavior in transition metal
oxides is indicative of there being rapid energy storage with no phase change, or, in rare cases, that the phase change occurs with a very small volume change between the charged and dis-charged phases. It should be noted that polarization processes will lead to peak voltage separation in all electrochemical systems; eqn (4) and (5) above are utilized in regions where the polarization is not signicant. For thin lms of transition metal oxides, this means that the experiment is performed at sweep rates of <100 mV s"1, and usually between 1 and 10 mV s"1.
In a constant current experiment, pseudocapacitance is indicated by a small voltage hysteresis between the charging and discharging steps. Since these materials do not undergo a phase transformation, the prole of potential vs. capacity will be almost linear in shape as described by eqn (2) and shown schematically in Fig. 8b as well as in the discharge curve for 6 nm LiCoO2nanocrystals in Fig. 9.
AC impedance can also be used to determine whether pseu-docapacitive behavior is taking place, although the interpretation of the impedance results is dependent upon the best equivalent circuit for the system. Furthermore, double-layer capacitance and pseudocapacitance may give similar impedance results. The Nyquist representation (real vs. imaginary impedance, Z) for an ideal capacitor is a vertical line, indicating a 90$ phase angle.
Deviation from a vertical line to phase angles of <90$oen occurs
and can indicate pseudocapacitive behavior, which is oen rep-resented by a constant-phase element in the equivalent circuit:39
here, Z is the impedance, B is a constant, u is the frequency, and
p is an adjustable constant. When p is 1, this corresponds to an
ideal capacitor and when p is 0.5, this indicates semi-innite diﬀusion. The impedance behavior of hydrous RuO2is shown in
Fig. 4 CV at 100 mV s"1of Au/MnO
2core–shell nanowires separated
into capacitive (varying with v) and diﬀusion (varying with v1/2)
contributions utilizing the analysis based on eqn (4). Reprinted with permission from ref. 33. Copyright 2012 American Chemical Society.
Fig. 5 Kinetic analysis of the capacity suggested by Trasatti et al. The example here is of NiCo2O4deposited on Ti with an interlayer of RuO2.
In the plot of capacity (q*) vs. v"1/2, the y-intercept corresponds to the inﬁnite sweep rate capacity, Qv¼N. Reprinted from ref. 35, with
permission from Elsevier.
Fig. 6 CV of Nb2O5 nanocrystals at 0.1 mV s"1in a non-aqueous
lithium ion electrolyte. At this rate, the peak voltages for lithium insertion/de-insertion overlap, a characteristic of materials which exhibit rapid energy storage kinetics.38
Fig. 7b. Analysis of impedance behavior has also been used to separate the double layer and pseudocapacitive contributions to charge storage in a mesoporous CeO2 electrode at diﬀerent
potentials in a non-aqueous lithium-ion electrolyte.40 It is
interesting to compare the impedance behavior of the meso-porous CeO2with that of hydrous RuO2. In the case of RuO2, the
Nyquist plots (Fig. 7b) are similar for a broad range of poten-tials, from 0.2 to 1.2 V. On the other hand, for mesoporous CeO2
(Fig. 7c), the impedance is potential-dependent due to the fact that in this material, the charge storage is due to potential-dependent Li+intercalation.
Materials that do not exhibit any of these electrochemical features are not pseudocapacitive, and it is questionable whether capacitance values should be used to characterize their electrochemical charge storage behavior. The electrochemical behavior of materials believed to be pseudocapacitive should be carefully analyzed to determine if pseudocapacitance is present. Fig. 8 summarizes the general electrochemical features of pseudocapacitive materials. In the following sections, the elec-trochemical behavior of various pseudocapacitive materials will be revisited and discussed in light of the key features presented above.
2.4. Intrinsic vs. extrinsic pseudocapacitance
Pseudocapacitance can be intrinsic to a material or extrinsic, in that the property can emerge through appropriate material
engineering. Regardless of whether a material is considered to be an intrinsic or extrinsic pseudocapacitor, it exhibits the features described in the prior section. Intrinsic pseudocapa-citive materials display the characteristics of capapseudocapa-citive charge storage for a wide range of particle sizes and morphologies. These are materials such as RuO2$nH2O,23MnO2,42and Nb2O5.38
On the other hand, extrinsic materials do not exhibit pseudo-capacitance in the bulk state due to phase transformations during ion storage. With these materials, increasing the surface area through nanostructuring leads to improved high-rate behavior due to a decrease in diﬀusion distances and in some cases, the suppression of a phase transformation. These two factors are exhibited by a number of transition metal oxides. For example, bulk LiCoO2exhibits a voltage plateau during lithium
insertion with an average voltage of about 3.9 V. Reducing the particle dimension to 17 nm or less reduces the voltage plateau in favor of a continuously sloping voltage prole over the entire intercalation range, with nanocrystals of 6 nm exhibiting an almost linear discharge curve (Fig. 9).43
Fig. 7 The utilization of AC impedance in analyzing pseudocapacitive behavior: (a) CVs of RuO2$0.5H2O in 0.5 M H2SO4and (b) Nyquist (complex
impedance) plot at diﬀerent potentials during the charging of RuO2$0.5H2O. The impedance results demonstrate that this material has relatively
small deviations from ideal capacitor behavior. (c) Results of the equivalent circuit ﬁtting of impedance data for mesoporous CeO2in 1 M LiClO4
in propylene carbonate. Reprinted with permission from (a & b) ref. 41 and (c) ref. 40. Copyright 2005 & 2010 American Chemical Society.
Fig. 8 The general electrochemical features of pseudocapacitive materials. (a) In a cyclic voltammetry experiment, the shape is rect-angular and if peaks are present, they are broad and exhibit a small peak-to-peak voltage separation. (b) In a galvanostatic experiment, the shape is sloping so that a capacitance value, DQ/DE, may be assigned at each point, and the voltage hysteresis is small. Here, Q is the capacity and E is the potential window. (c) In an AC impedance experiment, the Nyquist representation will contain a vertical line with a phase angle of 90$or less. A semi-circle at high frequencies,
asso-ciated with charge-transfer resistance, may also be present.
Fig. 9 The eﬀect of crystallite size on the lithiation (discharge) curve of LiCoO2measured for a 1 hour charge–discharge. For small crystallite
sizes the plateau region decreases and is replaced by a completely sloping voltage proﬁle. For 6 nm crystallites, the voltage proﬁle is almost linear in shape; this is due to the increased contribution of surface lithium ion storage sites. Reprinted with permission from ref. 43. Copyright 2007 American Chemical Society.
The change in behavior from a at discharge curve, as expected for a bulk material undergoing a phase transformation during a redox reaction, to a sloping one was attributed to the increased contribution of surface lithium ion storage sites in nanostructured LiCoO2. The site energy for an intercalated
lithium ion is expected to take on a range of values due to the structural disorder for the layers near the surface, and this translates to a discharge curve that is similar to the type described by eqn (2). As a result of the increased number of lithium storage sites near the surface, the rate capability of 17 nm nanocrystals was superior to that of bulk (!200 nm) LiCoO2. This
example demonstrates how pseudocapacitance can emerge when a material is engineered so that a large percentage of the lithium ion storage sites are limited to the surface by nano-structuring the material. In addition to LiCoO2, battery materials
that exhibit signicant pseudocapacitance when nanostructured include V2O5and nickel and cobalt hydroxides.
Materials that undergo crystallographic phase trans-formations during electrochemical cycling usually do not exhibit high rate behavior and there is a signicant voltage hysteresis between the charge and discharge steps. An example of this behavior is LiMn2O4, where the de-insertion/insertion of
lithium occurs between two distinct phases, the spinel LiMn2O4
and the metastable spinel l-MnO2, with an overall unit cell
volume change of 7.6%.44 The intercalation of lithium ions
within the spinel Li4Ti5O12is an exception to this trend because
here, the phase transformation occurs with zero strain.45This
unique behavior occurs due to the very close structural rela-tionship between the two diﬀerent phases, Li4Ti5O12 and
Li7Ti5O12, the latter being the fully lithiated phase, that results
in a volume change of less than 0.2%.46Electrodes of Li
nanocrystals with a diameter of 8 nm do not exhibit a sloping voltage plateau, suggesting that nanostructuring has little inuence on the lithium ion storage site energy, as can be expected from a two-phase system (Fig. 10). Thus far, it appears that Li4Ti5O12is the only material to exhibit the phenomenon of
zero-strain intercalation in a material that undergoes a phase change during lithiation. It is not a pseudocapacitive material as a capacitance cannot be dened at a voltage plateau.
Many transition metal oxides have been investigated for pseu-docapacitive charge storage in aqueous electrolytes. The behavior of these materials depends upon the structure of the material, hydration properties, and the electrolyte. The eﬀect of structural and surface-bound water is one major diﬀerence between aqueous and non-aqueous pseudocapacitive materials, as such structural water can result in a large “inner surface” that is available for ion adsorption, as in RuO2$nH2O. The structural
water may also aid in ion diﬀusion into the inner surface. Here, we will review the most important pseudocapacitive materials in aqueous electrolytes: MnO2, RuO2$nH2O, oxides with the
spinel structure such as Mn3O4, and transition metal
hydrox-ides. MnO2 exists in a number of polymorphs and most have
been investigated for pseudocapacitive behavior. Spinel oxides share a common structure but exhibit very diﬀerent behavior based on the transition metal(s) involved. Finally, the hydrox-ides exhibit extrinsic pseudocapacitance, as their battery-type behavior becomes increasingly pseudocapacitive with nano-structuring. MnO2, the most widely studied pseudocapacitor
material, is reviewed rst. 3.1. MnO2
The pseudocapacitive behavior of MnO2was rst investigated in
1999 by Lee and Goodenough as they studied the properties of amorphous MnO2$nH2O in a KCl aqueous electrolyte.48 The
presence of a rectangular voltammogram and the storage of approximately 200 F g"1(240 C g"1, 4 min) indicated that rapid faradaic reactions were responsible for charge storage in this material, as shown in Fig. 11a. In general, pseudocapacitive charge storage of MnO2 in an aqueous electrolyte occurs
through the redox of Mn between the +4 and +3 oxidation states at the surface or in the bulk:49
MnO2+ xA++ xe"4 AxMnO2 (7)
here, A represents an alkali metal cation. Theoretically, the 1-electron redox reaction (x ¼ 1) corresponds to 1233 F g"1(1110
C g"1) assuming a 0.9 V potential window. MnO
and low cost, which makes it particularly appealing when compared to RuO2. However, MnO2does not possess the high
electronic conductivity of RuO2 (104 S cm"1 for bulk single
crystal): depending on the crystal structure, the conductivity of MnO2ranges from 10"7 to 10"3S cm"1.50As a result, charge
storage in MnO2occurs within a thin layer of the surface.49This
translates into capacitance values that are signicantly lower from the theoretical value for thick composite electrodes, where typical specic capacitances range between 200 and 250 F g"1,
while still exhibiting the pseudocapacitive electrochemical signature in cyclic voltammetry or galvanostatic experiments. On the other hand, it has been shown that ultrathin lms of MnO2 can achieve specic capacitances of >1000 F g"1,33,49
demonstrating that nanostructuring is a highly eﬀective method for accessing all of the MnO2storage sites. The various
Fig. 10 Charge–discharge curve of nanocrystalline (5–20 nm) Li4Ti5O12attached to carbon nanoﬁbers cycled at a 1 hour charge–
discharge time. Unlike in LiCoO2, nanostructuring does not lead to a
sloping voltage proﬁle. Reprinted from ref. 47, with permission from Elsevier.
strategies being developed for MnO2 electrodes for
electro-chemical capacitors have been reviewed.51
Both amorphous and crystalline forms of MnO2have been
investigated for high-rate energy storage in aqueous electro-lytes. It has been suggested that charge storage in amorphous MnO2takes place mainly on the surface, while crystalline MnO2
has an additional capacitive contribution from bulk ion inter-calation.52However, experimental results demonstrate that in
both amorphous and crystalline materials, a high BET surface area does not necessarily lead to high capacitance suggesting that in both types of materials, ions insert into sub-surface sites. Brousse et al.42plotted the specic capacitance for a number of
crystalline and amorphous MnO2compounds as a function of
surface area. In the case of amorphous materials, the average capacitance was around 160 F g"1. Crystalline materials exhibit capacitance values up to !250 F g"1, a bit higher than the amorphous materials, and the fact these are achieved with lower surface areas is indicative of a greater contribution of faradaic reactions to these materials.
The structural chemistry of crystalline MnO2is very rich, and
there are many allotropes. Two diﬀerent studies50,53reported the
eﬀects of crystal structure on the capacitance of MnO2 in
aqueous electrolytes (using thick composite electrodes). Both concluded that a wide intercalation tunnel contributes to high capacitance values and that a high BET surface area does not necessarily lead to the best performance. The capacitance as a function of cycle number for diﬀerent MnO2allotropes is shown
in Fig. 11b. Ghodbane, et al. found the highest capacitance with the spinel form (l-MnO2; 245 F g"1; 196 C g"1, !2.67 min) while
Devaraj et al. found the highest capacitance with hollandite MnO2(a-MnO2; 297 F g"1; 297 C g"1; !5 min). The diﬀerent
ndings are likely due to the use of diﬀerent synthesis and electrochemical characterization methods.54
It is well-known that Mn3+formed during the redox process disproportionates under acidic, and even near-neutral, condi-tions.51This can limit the lifetime of devices that utilize MnO
electrodes. The loss of capacity can be partially mitigated by appropriate electrode and/or cell engineering. For example, by increasing the binder content, thick composite electrodes exhibited only a 5.8% capacity fade over 1000 cycles at a specic current of 2 A g"1(!7.5 s).55Removing dissolved oxygen from
the electrolyte also leads to a marked improvement in the MnO2
MnO2 exhibits electrochemical features representative of
intrinsic pseudocapacitive charge storage. The low cost, abun-dance, and high theoretical capacitance makes it a very attrac-tive material for aqueous-based electrochemical capacitors. The main challenge for this material is to improve its poor elec-tronic conductivity in order to access the full theoretical capacitance in thick lms and at high rates.
As mentioned previously, hydrous RuO2was the rst material to
demonstrate pseudocapacitance. While its scarcity and high cost are prohibitive for large-scale applications, there have been signicant eﬀorts in fabricating advanced electrodes due to its excellent properties. The motivation for these studies has been to utilize the RuO2as eﬃciently as possible by achieving the
maximum theoretical capacitance and using as little of the RuO2 as possible. For example, the traditional slurry method
with a high RuO2$nH2O mass loading of !30 mg cm"2results in
a capacitance of 720 F g"1for a charge–discharge time of !8
minutes.23This is approximately 50% of the theoretical
capac-itance of RuO2$nH2O. Utilizing RuO2nanoparticles dispersed
onto activated carbon (10 wt% RuO2$nH2O/90 wt% activated
carbon) leads to capacitances of 1340 F g"1 for charge–
discharge times of !1 minute,57which is much closer to the
expected theoretical value. This increase in the capacitance and rate occurs due to the very eﬀective exposure of the RuO2$nH2O
to the electrolyte. The drawback to this type of electrode archi-tecture is of course that the total mass loading of RuO2$nH2O
per footprint area is low, leading to low areal capacitance values. 3.3. Oxides with the spinel structure
The spinel crystal structure, with a general formula AB2O4, is
very important for EES. It oﬀers a robust crystalline architecture with three dimensional diﬀusion pathways. A number of spinel compounds have been investigated for electrochemical capaci-tors, including Mn3O4,58Fe3O4,59and Co3O4,60along with mixed
transition metal spinels such as MnFe2O4,61and NiCo2O4.62Of
these, Mn3O4, Fe3O4, and MnFe2O4 exhibit the characteristic
Fig. 11 (a) CV at 5 mV s"1of a thick composite electrode of amorphous MnO2$nH2O in 2 M KCl electrolyte. At this sweep rate, the capacitance
was!200 F g"1. Reprinted from ref. 48, with permission from Elsevier. (b) The speciﬁc capacitance and cyclability of diﬀerent MnO
under investigation for high-rate energy storage as tested in a composite electrode architecture in 0.5 M K2SO4electrolyte at 5 mV s"1. Reprinted
pseudocapacitive features presented in Fig. 8, including mostly rectangular CVs.
As with MnO2, the poor electronic conductivity of Mn3O4
leads to low capacitance values for thick electrodes and large particle sizes. For a 1.2 mm-thick electrode of Mn3O4particles
(120–140 nm), the cyclic voltammogram is rectangular with a maximum capacitance of 314 F g"1(314 C g"1; 3.3 min).63The
addition of an eﬀective electronically conductive scaﬀold material such as graphene improves the rate capability at the expense of the specic capacitance, which decreases to 120 F
g"1when the mass of the scaﬀold is included.58The mechanism
of pseudocapacitive charge storage in Mn3O4 is not fully
established. Recent in situ X-ray absorption near-edge spectra (XANES) experiments have shown that, in a Na2SO4electrolyte,
the mechanism involves the reversible redox of Mn3+to Mn2+.64
In that study, the highest observed capacitance was 261 F g"1
(235 C g"1; 15 min) for Mn
3O4 nanocrystal-lm electrodes. A
larger capacitance value for Mn3O4was found to occur by using
a carbon nanotube conductive architecture with KCl electrolyte. In this case, the specic capacitance was 420 F g"1(294 C g"1; 2.33 min).65
Only a few reports describe the pseudocapacitive behavior of MnFe2O4and Fe3O4as the capacitance values of these materials
are modest. Crystalline MnFe2O4 contained in a thick
composite electrode architecture exhibits capacitance values of approximately 105 F g"1 (94.5 C g"1, 45 s) in a NaCl electro-lyte.61,66 Its pseudocapacitive mechanism is not clear but is
believed to involve redox reactions occurring with both Mn and Fe, according to in situ XANES of Mn and Fe K-edges.61In Fe
the redox process has been ascribed to the adsorption of anions and the capacitance has been found to be approximately 170 F
g"1(119 C g"1, 5.8 min) for thin lms in Na2SO3electrolyte.59
Co3O4,60NiCo2O4,67and MnCo2O468diﬀer from the behavior
of the spinel materials described above since they can exhibit battery-type behavior due to the formation of oxyhydroxides during the charge storage process. As shown in Table 1, the reported capacitance values for these materials are signicantly larger. This is due to the formation of transition metal oxy-hydroxides during the charging process in an alkaline electro-lyte, where M indicates Ni, Co, or a combination of these:67
M3O4+ OH"+ H2O 4 3MOOH + e" (8)
This two-phase reaction (eqn (8)) involves one phase trans-formation, which results in a constant potential during galva-nostatic charge–discharge and also limits the rate capability.
However, when M ¼ Co, the electrochemically formed oxy-hydroxide participates in a second reversible redox process:
CoOOH + OH"4 CoO2+ H2O + e" (9)
Fig. 12 demonstrates the presence of several sets of broad redox peaks that have been ascribed to such reactions in Co3O4.
Thus, the electrochemical signature of these materials combines pseudocapacitive (eqn (9)) and battery (eqn (8)) contributions.
NiCo2O4exhibits particularly high capacitance values even at
short charge–discharge times. This appears to be due to the combination of good electronic conductivity in the discharged material, !62 S cm"1, and utilizing the redox behavior of both
nickel and cobalt.67The energy storage properties for NiCo
have been ascribed to the reversible transformation of the parent spinel compound into nickel and cobalt oxyhydroxides. The cobalt oxyhydroxide is then believed to undergo a second reversible redox reaction, as shown in eqn (9). The theoretical capacity for this overall 3-electron process (per NiCo2O4),
including both the pseudocapacitive and the battery-like fara-daic contributions, is 1203 C g"1 or 2005 F g"1 assuming a typical 0.6 V potential window in an aqueous alkaline electro-lyte. Values close to the theoretical capacitance can be achieved Table 1 Capacitance values of spinel oxides where an oxyhydroxide phase participates in the charge storage mechanism
Material Capacitance (F g"1) Capacity (C g"1) Charge–discharge time (s)
Active material mass
loading (mg cm"2) Reference
Co3O4 382 229 115 0.5 60
NiCo2O4 1400 672 19 0.4 71
678 339 339 8 67
MnCo2O4 346 173 173 1 68
Fig. 12 CVs for a composite electrode consisting of Co3O4nanowires
in 1 M KOH from 5 to 50 mV s"1. The inset shows the linear
depen-dence of the anodic peak on the sweep rate, indicative of pseudo-capacitive behavior. Reprinted with permission from ref. 69. Copyright 2011 American Chemical Society.
by using electrode architectures in which NiCo2O4nanosheets
are electrodeposited onto carbon nanobers.70
The spinel materials described above exhibit both capacitive and battery-type behavior due to the phase changes involved in the cycling process. The preparation of these materials in nanoscale form is expected to emphasize the pseudocapacitive contribution. Thus, in order to improve our understanding of charge storage in these materials, it is important to use the various analyses of kinetics to separate capacitive and diﬀusion contributions.
3.4. Nanostructured layered metal hydroxides
The hydroxides of divalent transition metal oxides, M2+(OH) 2,
tend to form lamellar structures that generally consist of MO6
octahedra separated by hydrogen atoms.72When some of the
transition metals are present in the +3 state, the additional positive charge of the slabs can be compensated by the inter-calation of anion species into the interlayer spacing, forming a layered double hydroxide.73 In the hydroxides, the interlayer
spacing is several nm74and allows for the reversible
intercala-tion of ions. The nickel and cobalt transiintercala-tion metal hydroxides are an important class of materials that have found commercial application as electrodes in rechargeable aqueous batteries.75
Charge storage in these materials involves at least one phase transformation, which results in a constant potential during galvanostatic charge–discharge and also limits the rate capa-bility. Section 2.4 described how pseudocapacitive behavior can emerge when battery materials are nanostructured and energy storage takes place at or near the surface. As a result, nano-structured hydroxides have been investigated as pseudocapa-citive electrodes for electrochemical capacitors. These hydroxides can be considered as extrinsic pseudocapacitors as the bulk materials exhibit battery-type behavior.
Charge storage in Ni(OH)2occurs via reversible redox of the
Ni2+/Ni3+couple in an alkaline electrolyte, typically KOH:
Ni(OH)2+ OH"4 NiOOH + H2O + e" (10)
This reaction corresponds to a theoretical capacity of 1040 C
g"1within a 0.5 V potential window. In a suitably nanostructured
material, a maximum specic capacitance of 2080 F g"1would be
possible. In bulk form, the reaction gives rise to a single pair of redox peaks, which occur at approximately 0.36 V (vs. Ag/AgCl) for the oxidation and 0.26 V for the reduction.76Fig. 13 shows a
qualitative comparison between the charge–discharge proles of a bulk Ni(OH)2electrode (Fig. 13a) that exhibits a battery-type
potential plateau and a nanostructured electrode (Fig. 13b) which has both a potential plateau and sloping potential regions. The sloping regions at potentials above and below !0.35 V likely correspond to pseudocapacitive contributions from surface or near-surface charge storage. The capacitance of the nanostructured Ni(OH)2was found to be as high as 1750 F g"1,
although this value was calculated over the entire potential region, including the battery-type plateau. While the specic capacitance of Ni(OH)2can be larger than that of RuO2or MnO2,
it occurs over a smaller potential window.
Co(OH)2can also be cycled in an alkaline electrolyte where
the charge storage takes place via reversible redox between Co2+/ Co3+ states. The pseudocapacitive properties of cobalt hydroxide in nanostructured form are not as well explored but appear similar to Ni(OH)2. As with Ni(OH)2, there is a single pair
Fig. 13 Comparison of the charge–discharge proﬁles of Ni(OH)2in (a) bulk (reproduced from ref. 77 by permission of The Electrochemical
Society) and (b) nanostructured forms. The nanostructured electrode contains both the ﬂat battery-type potential region along with sloping pseudocapacitive regions. Reproduced from ref. 78 with permission from The Royal Society of Chemistry.
Fig. 14 CVs at various sweep rates for electrodeposited Co(OH)2on
graphene nanosheets. The electrochemical behavior was performed using three-electrode cells in 1 M KOH electrolyte. Reproduced from ref. 79 with permission from Elsevier.
of redox peaks over a 0.5 V potential window.79Fig. 14
demon-strates that when nanostructured, Co(OH)2exhibits good peak
overlap and thus high rate capability. Very high specic capacitances have been reported, up to 2646 F g"1(1455 C g"1in !3 min).80 However, as with Ni(OH)
2, this capacitance value
oen includes contributions from battery-type behavior.
3.5. High-rate performance of aqueous electrolyte pseudocapacitive materials
In this section, the high-rate performance of diﬀerent aqueous pseudocapacitive materials is examined. We focus on those studies that demonstrate a charge–discharge time of !1 minute. This is relevant for practical device considerations: at timescales greater than about 10 minutes, advanced lithium-ion batteries may be able to provide higher energy densities. Mass loading and electrode porosity greatly inuence the rate capa-bility. Designing high-rate electrodes with high active material mass loading and optimum porosity to allow electrolyte access at high rates and suﬃcient electronic conductivity remains a challenge for all pseudocapacitive materials.
High rate studies have been carried out on several polytypes of MnO2. a-MnO2(hollandite) powders in traditional composite
electrode architectures (200 mm electrode thickness; 80 wt% active material mass loading) exhibit a capacitance value of 166
F g"1 at a sweep rate of 2 mV s"1, which corresponds to a
charge–discharge time of 7.5 minutes.81 At a sweep rate of
20 mV s"1(t ¼ 45 s), the capacitance decreases by 40% to 100 F
g"1. Depositing MnO2 onto a conductive substrate such as
carbon nanotubes,82,83graphene,84and carbon foam85or
form-ing a thin lm49allows for better exposure of the MnO
to the electrolyte and mitigates its poor electronic conductivity. For example, when g-MnO2(nsutite) was electrodeposited onto
carbon nanotubes with a mass loading of !0.05 mg cm"2, at a sweep rate of 50 mV s"1(t ¼ 20 s), the capacitance was !490 F
g"1over a 1 V potential window.83Moreover, the current density
as a function of the sweep rate was found to be linear from 10 to 150 mV s"1conrming that the charge storage was
pseudoca-pacitive over a wide timescale. However, 490 F g"1is still less
than 50% of the expected theoretical capacitance of MnO2.
There are several studies reporting very good rate capabilities for the high-capacitance spinel oxides, MnCo2O4and NiCo2O4,
and the hydroxides Ni(OH)2 and Co(OH)2. For example, at a
high active material mass loading of 8 mg cm"2and utilizing a traditional composite electrode architecture, the capacitance of NiCo2O4was found to be 630 F g"1for a charge–discharge time
of 1 minute.67Amorphous Ni(OH)
onto graphite, with a mass loading of 0.12 mg cm"2, give a very high extrinsic capacitance of 1500 F g"1at a charge–discharge time of 1 minute.86The challenge with these materials is not
only to achieve a high specic capacitance at a short timescale, but also to broaden their typical 0.5 V potential window and decrease the battery-type plateau regions that occur due to phase transformations and thus limit kinetics.
Recent studies have shown good high-rate capability in materials that have not been widely investigated for pseudoca-pacitive behavior in aqueous electrolytes. A composite of MoO3,
CNTs, and activated carbon (where MoO3accounted for 10% of
the mass) exhibited a capacitance of 270 F g"1for over 10 000
cycles at a 4 minute charge–discharge rate.87The MoO
loading was selected so that the oxide was mostly encapsulated within the carbon matrix in order to prevent degradation during cycling. Tungsten oxide (WO3) is interesting for electrochemical
capacitors due to its good electronic conductivity when synthesized in a partially reduced form and within a conductive carbon network.88However, the gravimetric capacitance is low
(!103 F g"1; 16 min) mostly due to the weight of tungsten.
Some materials exhibit pseudocapacitive behavior in non-aqueous lithium-ion and, occasionally, sodium-ion electrolytes. Materials that exhibit pseudocapacitance do so because ion insertion induces a redox reaction which maintains charge neutrality. They may also have structures that support fast ion insertion. Since the electrolytes are non-aqueous, structural water no longer acts as a benecial ion-conducting pathway as in aqueous pseudocapacitive materials; rather, it can lead to the degradation of the electrochemical cell.89 One advantage for
using pseudocapacitive materials in non-aqueous electrolytes is that they typically exhibit capacitance over wider potential ranges than materials in aqueous electrolytes as:
here, E is energy density (J g"1), C is the capacitance (F g"1), and
V is the potential range (V). Thus, by widening the potential
range from 1 to 4 V, the energy density can increase by nearly an order of magnitude. From a mechanistic standpoint, one is able to separate pseudocapacitance and double-layer capacitance by judiciously selecting electrolytes whose bulky ions will prevent ion insertion.90 In the paragraphs below we review materials
systems in which ion insertion from non-aqueous electrolytes gives rise to pseudocapacitive charge storage.
4.1. Amorphous materials
Amorphous materials exhibit single-phase ion intercalation behavior, and so their charge–discharge behavior may be rep-resented by eqn (2). Some crystalline materials may become amorphous with repeated electrochemical cycling or by the intercalation of ions past a certain composition, as detailed for V2O5in the next section. The structural disorder of amorphous
materials can be benecial for EES,91although sometimes these
materials will exhibit lower capacities than their crystalline counterparts. Whether amorphous materials are benecial for pseudocapacitive EES depends upon their high rate capability. Amorphous MoO331and Nb2O5,92for example, exhibit lower
capacitances than their crystalline counterparts even at short charging times and in a thin lm conguration. These results suggest that the crystalline materials possess better kinetics and/or another charge storage mechanism which leads to higher specic capacitance. On the other hand, amorphous
TiO2 nanotubes exhibit an interesting transformation to an
ordered cubic phase when cycled in a lithium-ion electrolyte.93
This material exhibits high rate capability and capacity, and the charge–discharge curves appear like those expected for solid-solution type behavior.
Vanadium oxides form layered structures which are very advantageous for EES. There is a rich structural chemistry associated with these materials due to the large number of oxidation states of vanadium. A recent review describes a number of these materials.94 V
2O5 is very attractive for EES
because the high oxidation state of vanadium leads to the possibility of storing more than 1 electron per formula unit (+5, +4, +3, and +2 are electrochemically accessible) and the ability to form layered compounds. When in the bulk, crystalline (orthorhombic) form (Fig. 15a), V2O5does not exhibit capacitive
behavior and there are several well-dened voltage plateaus corresponding to diﬀerent lithiation phases.95 Bulk
ortho-rhombic V2O5 is limited to the storage of one lithium per
formula unit before the onset of an irreversible phase trans-formation.94Lithiation can proceed until the formation of the
rock-salt u-Li3V2O5 phase at approximately 1.8 V vs. Li/Li+.
Further lithiation of the bulk crystalline material at lower potentials results in structural degradation.96,97
Both amorphous and nanocrystalline forms of V2O5 can
exhibit pseudocapacitive behavior as evidenced by sloping charge–discharge curves during galvanostatic cycling and broad, featureless CVs. One unique class of these materials is synthe-sized from a V2O5gel99into xerogels,100ambigels,101or aerogels90
depending on the solvent removal technique. The structure of V2O5xerogels (Fig. 15b) consists of V2O5bilayers separated from
each other by a large van der Waals gap of !12 ˚A that contains water molecules in the as-synthesized state.102 Locally, the
structure of the ambigels and aerogels is expected to be similar to the xerogels; the large van der Waals gap is preserved in these materials and its size ranges from 10–14 ˚A depending on the amount of structural water present. This large van der Waals gap allows for the insertion of a large variety of cations.103,104The
galvanostatic cycling of xerogel and amorphous V2O5is shown in
Fig. 16 and compared to that of bulk orthorhombic V2O5.
The pseudocapacitance of high surface area V2O5is strongly
dependent upon exposure of the active material to the electrolyte.
This behavior is one characteristic of an extrinsic pseudocapa-citor material. For example, V2O5 aerogels exhibit almost
perfectly capacitive CVs when analyzed using the 'sticky carbon' method in which a small amount of the aerogel (surface area of 280 m2g"1) material is pressed into a conductive wax (Fig. 17).90
In such an electrode architecture, nearly all of the active material surface area can be exposed to the electrolyte. The maximum capacitance of V2O5aerogels was determined to be 1300 F g"1
(1820 C g"1; 3.9 h).90On the other hand, an aerogel electrode
made using the traditional composite electrode technique exhibits a CV with prominent intercalation peaks. This has been ascribed to the increased crystallization of the aerogel material that occurs during the heat treatment required for fabricating a composite electrode.
Nanocrystalline V2O5can also exhibit signicant
pseudoca-pacitive behavior. The poor electronic conductivity of V2O5must
be overcome with the use of an appropriate conductive material Fig. 16 Galvanostatic cycling of (a) orthorhombic V2O5, (b) V2O5
xerogel, and (c) amorphous V2O5. Reprinted from ref. 105, with
permission from Elsevier.
Fig. 15 Two types of layered sheet structures of V2O5: (a) the structure
of orthorhombic V2O5(reproduced from ref. 95 with permission from
Elsevier) and (b) the layered structure of V2O5xerogels. Reprinted by
permission from Macmillan Publishers Ltd: Nat. Mater., ref. 98, copy-right 2003.
Fig. 17 Cyclic voltammetry of a V2O5aerogel electrode at 5 mV s"1
using the sticky carbon electrode. The dotted CV represents the sticky carbon background current. Reproduced with permission from ref. 90. Copyright 2000, The Electrochemical Society.
for fast kinetics. V2O5 nanowires entangled with CNTs, for
example, exhibit capacitive CVs in sodium-ion non-aqueous electrolyte.106 Deposition of V
2O5 layers onto CNTs has been
performed using atomic layer deposition (ALD),107
electrode-position,108 and hydrolysis.32 These studies further
demon-strated the importance of exposing as much of the material as possible to the electrolyte for the highest capacitance values. Moreover, the extrinsic pseudocapacitive nature of the V2O5was
evident as increasing the V2O5 layer thickness resulted in a
decrease in the capacitance value, as well as the transition from capacitive to battery-like electrochemical features. This behavior is illustrated in Fig. 18 for V2O5 that was deposited
during an in situ chemical hydrolysis of a vanadium precursor. The separation of diﬀusion-controlled and capacitive currents was performed using the current-separation technique described by eqn (4).
Nanostructured V2O5materials are promising for high-rate
EES storage. As an extrinsic pseudocapacitor, exposure of the surface area to the electrolyte is critical. Moreover, increasing the thickness of the material leads to a decrease in the pseu-docapacitive behavior. To build high-rate electrodes, the poor electrical conductivity of V2O5 must be overcome with
appro-priate conductive supports. In addition, vanadium dissolution is possible and care should be taken to avoid the use of elec-trolytes that can have even trace amounts of acid as these have been shown to severely limit the life cycle of V2O5electrodes.109
4.3. TiO2(B) and hydrogen titanates
Hydrogen titanates, primarily H2Ti3O7, and TiO2(B) have been
investigated for pseudocapacitive EES. In these materials, as in other titanium oxides, charge storage occurs due to the Ti +4/+3 redox couple, and lithium ion intercalation occurs below 2 V vs. Li/Li+. The hydrogen titanates are layered structures consisting of edge-sharing TiO6 octahedra separated by protons; heat
treatment of these materials leads to dehydration and the formation of the TiO2(B) phase, which consists of two
edge-sharing TiO6 octahedra linked at corners110 (as shown in
Fig. 19). The resulting TiO2material has a lower density111and
therefore a more open structure than anatase or rutile phases of TiO2, which makes it interesting for pseudocapacitive energy
Investigations of the electrochemical behavior of hydrogen titanates in lithium ion non-aqueous electrolytes have shown that the charge storage is pseudocapacitive in nature. These investigations have been primarily carried out on nano-structured materials such as nanowires and nanotubes.113–117
The materials exhibit the electrochemical features of pseudo-capacitance, as shown in Fig. 20 for H2Ti3O7 nanowires. A
reversible capacity of 597 C g"1(!398 F g"1; !5 min) has been obtained with a composite electrode composed of hydrogen Fig. 19 The structures of (a) H2Ti3O7 and (b) TiO2(B) as viewed
perpendicular to the (010) plane. Reproduced from ref. 112 by permission of IOP Publishing.
Fig. 18 Total charge storage of V2O5 (at 0.1 mV s"1) chemically
deposited onto CNTs, separated into contributions from intercalation (diﬀusion-controlled current) and capacitance for diﬀerent V2O5
thicknesses, represented by diﬀerent loading %. Reprinted with permission from ref. 32. Copyright 2011 American Chemical Society.
Fig. 20 (a) CVs of H2Ti3O7nanowires in a non-aqueous lithium ion electrolyte; (b) the dependence of the peak current with sweep rate is linear
titanate nanotubes in which the active material mass loading was 3–4 mg cm"2.114The pseudocapacitive behavior of hydrogen
titanates has been attributed to the increased surface area of the nanostructured materials as well as the large interlayer spacing of the titanates, !8 ˚A.113
The electrochemical behavior of TiO2(B) is also
pseudoca-pacitive in nature, as rst reported by Zukalov´a, et al.111Charge
storage in TiO2(B) occurs via the intercalation of lithium ions in
a non-aqueous electrolyte:
TiO2(B) + xLi++ xe"4 LixTiO2(B) (12)
It is understood that some lithium remains in the material aer the rst cycle so that TiO2(B) is not recovered.118 The
theoretical capacity for a full 1 electron redox reaction is 335 mA
h g"1(1206 C g"1). In a CV, TiO2(B) exhibits two sets of cathodic
redox peaks, at !1.5 and 1.6 V, which are located at lower potentials than for lithium ion intercalation into anatase TiO2
(!1.75 V). In bulk TiO2(B), these peaks exhibit a linear
depen-dence on the sweep rate indicative of a pseudocapacitive process.111The material may also be synthesized in nanosheet
and nanowire forms, and their electrochemical behavior is slightly diﬀerent;119
in both cases, however, the charge– discharge proles are sloping as shown in Fig. 21. The pseu-docapacitive behavior of TiO2(B), which is diﬀerent from other
forms of TiO2, has been ascribed to the low-density crystal
structure that contains channels for rapid lithium ion transport from the surface to the sub-surface.111Nanostructuring, in the
form of nanowires, nanosheets, and nanoparticles, decreases the ion diﬀusion distance and thus increases the rate capability even further.118 For example, TiO
2(B) nanosheets exhibit
capacities of 777 C g"1(518 F g"1) in !3.9 min.120
The hydrogen titanates and TiO2(B) are examples of intrinsic
pseudocapacitors. They exhibit broad, overlapping redox peaks in CVs and continuously sloping charge–discharge curves, even in bulk form. Further studies are needed to fully characterize the rate-capability of these materials, particularly at timescales of 1 minute or less. Unlike in V2O5, exposure of the surface to
the electrolyte is not critical as thick composite electrodes exhibit pseudocapacitive behavior. A major concern with these materials is that nanostructured forms, which show higher capacity and rate capability than the bulk, exhibit irreversible capacity loss during cycling.
While the electrochemical energy storage capabilities of Nb2O5
have been known since 1980,121,122only recently has the
pseu-docapacitive behavior of orthorhombic T-Nb2O5 been
identi-ed.38,92,123In general, the charge storage of T-Nb
to the insertion of lithium ions in non-aqueous electrolytes at a potential of <2 V vs. Li/Li+. Based on the redox of the Nb +5/+4 couple, charge storage occurs up to 2 Li+/Nb2O5for a maximum
capacity of 720 C g"1.124The pseudocapacitive behavior is highly
dependent upon the presence of a crystalline structure. Amor-phous Nb2O5exhibits lower specic capacitance values (262 F
g"1; 314 C g"1; 4 min) than T-Nb2O5(555 F g"1; 666 C g"1; 4
min) despite the fact that the amorphous material has a much Fig. 21 Galvanostatic charge–discharge plots of TiO2(B) nanosheets
(NS) and nanoparticles (NP) at current density of 25 mA g"1. Reprinted with permission from ref. 119. Copyright 2012 American Chemical Society.
Fig. 22 (a) CVs of T-Nb2O5from 100–500 mV s"1exhibit broad, highly reversible redox peaks. (b) The peak cathodic and anodic currents scale